 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          
'K2 B18 V12 O54 (O H)6 (H2 O) [K8 (H2 O)16], 3(H2 O)' 
_chemical_formula_sum 
 'B18 H46 K10 O80 V12' 
_chemical_formula_weight          2523.18 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'B'  'B'   0.0013   0.0007 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            triclinic 
_symmetry_space_group_name_H-M    'P -1'  
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    11.901(12) 
_cell_length_b                    13.365(14) 
_cell_length_c                    13.987(14) 
_cell_angle_alpha                 117.070(11) 
_cell_angle_beta                  96.342(12) 
_cell_angle_gamma                 107.344(13) 
_cell_volume                      1810(3) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        BLOCK 
_exptl_crystal_colour             RED 
_exptl_crystal_size_max           0.21 
_exptl_crystal_size_mid           0.17 
_exptl_crystal_size_min           0.11 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.272 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1196
_exptl_absorpt_coefficient_mu     2.189 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.5957 
_exptl_absorpt_correction_T_max   0.7517 
_exptl_absorpt_process_details     
 'Jacobson, R. (1998) Private communication' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Rigaku Mercury'
_diffrn_measurement_method        ω
_diffrn_detector_area_resol_mean  7.31
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             9777 
_diffrn_reflns_av_R_equivalents   0.0180 
_diffrn_reflns_av_sigmaI/netI     0.0333 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -12 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -16 
_diffrn_reflns_limit_l_max        14 
_diffrn_reflns_theta_min          1.71 
_diffrn_reflns_theta_max          25.10 
_reflns_number_total              6321 
_reflns_number_gt                 5443 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1112P)²+20.1182P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.' 
_refine_ls_hydrogen_treatment     NONE
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          6321 
_refine_ls_number_parameters      551 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0753 
_refine_ls_R_factor_gt            0.0669 
_refine_ls_wR_factor_ref          0.2009 
_refine_ls_wR_factor_gt           0.1924 
_refine_ls_goodness_of_fit_ref    1.048 
_refine_ls_restrained_S_all       1.048 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
V1 V 0.43054(10) 0.79477(10) 0.70738(9) 0.0154(3) Uani 1 1 d . . . 
V2 V 0.37449(10) 0.65860(10) 0.83045(9) 0.0149(3) Uani 1 1 d . . . 
V3 V 0.64716(10) 0.79629(10) 0.91768(9) 0.0146(3) Uani 1 1 d . . . 
V4 V 0.82891(10) 1.05403(10) 1.07859(9) 0.0140(3) Uani 1 1 d . . . 
V5 V 0.72799(10) 1.05390(10) 0.87078(9) 0.0142(3) Uani 1 1 d . . . 
V6 V 0.50007(10) 1.05334(10) 0.75712(9) 0.0154(3) Uani 1 1 d . . . 
K1 K 0.94367(16) 0.82511(18) 1.03119(17) 0.0352(4) Uani 1 1 d . . . 
K2 K 0.55125(19) 0.46996(18) 0.82982(17) 0.0389(5) Uani 1 1 d . . . 
K3 K 0.6496(3) 0.1767(3) 0.5424(3) 0.0829(10) Uani 1 1 d . . . 
K4 K 0.08159(19) 0.41328(19) 0.75038(16) 0.0411(5) Uani 1 1 d . . . 
K5 K 0.2376(4) 0.4738(4) 0.5197(4) 0.1028(12) Uani 1 1 d . . . 
O1 O 0.7161(5) 0.7037(4) 0.8720(4) 0.0248(11) Uani 1 1 d . . . 
O2 O 0.8339(5) 1.0692(5) 0.8083(4) 0.0249(11) Uani 1 1 d . . . 
O3 O 0.3363(5) 0.5136(5) 0.7500(4) 0.0267(12) Uani 1 1 d . . . 
O4 O 0.9701(4) 1.0683(5) 1.0977(4) 0.0242(11) Uani 1 1 d . . . 
O5 O 0.5104(5) 1.0627(5) 0.6468(4) 0.0284(12) Uani 1 1 d . . . 
O6 O 0.5096(4) 0.7220(4) 0.9592(4) 0.0177(10) Uani 1 1 d . . . 
O7 O 0.1769(4) 0.8378(4) 0.7686(4) 0.0163(10) Uani 1 1 d . . . 
O8 O 0.4153(4) 1.1623(4) 0.8373(4) 0.0164(10) Uani 1 1 d . . . 
O9 O 0.6461(4) 1.1624(4) 0.8809(4) 0.0174(10) Uani 1 1 d . . . 
O10 O 0.2587(4) 0.6720(4) 0.9262(4) 0.0159(10) Uani 1 1 d . . . 
O11 O 0.8088(4) 1.1631(4) 1.0310(4) 0.0180(10) Uani 1 1 d . . . 
O12 O 0.2954(4) 0.7158(4) 0.7501(4) 0.0184(10) Uani 1 1 d . . . 
O13 O 0.5740(4) 0.9401(4) 0.7554(4) 0.0176(10) Uani 1 1 d . . . 
O14 O 0.2690(4) 1.0911(4) 0.9226(4) 0.0185(10) Uani 1 1 d . . . 
O15 O 0.5111(4) 0.7436(4) 0.7939(4) 0.0188(10) Uani 1 1 d . . . 
O16 O 0.3569(4) 0.9093(4) 0.7158(4) 0.0188(10) Uani 1 1 d . . . 
O17 O 0.7389(4) 0.9422(4) 0.9184(4) 0.0186(10) Uani 1 1 d . . . 
O18 O 0.4104(5) 0.7028(5) 0.5759(4) 0.0271(12) Uani 1 1 d . . . 
O19 O 0.2270(4) 1.2018(4) 0.8383(4) 0.0194(10) Uani 1 1 d . . . 
O20 O 0.2117(4) 0.9999(4) 0.7236(4) 0.0163(10) Uani 1 1 d . . . 
O21 O 0.1586(5) 0.7982(4) 0.5787(4) 0.0209(10) Uani 1 1 d . . . 
O22 O 0.8054(4) 1.3486(4) 0.9221(4) 0.0209(10) Uani 1 1 d . . . 
O23 O 0.1019(4) 0.6574(4) 0.7878(4) 0.0168(10) Uani 1 1 d . . . 
O24 O 0.9484(4) 1.3509(5) 1.0568(4) 0.0207(10) Uani 1 1 d . . . 
O25 O 0.6104(4) 1.3455(4) 0.9384(4) 0.0167(10) Uani 1 1 d . . . 
O26 O 0.2440(5) 1.4051(5) 0.9221(5) 0.0278(12) Uani 1 1 d . . . 
O27 O 0.4227(4) 1.3666(4) 0.9428(4) 0.0198(10) Uani 1 1 d . . . 
O28 O 1.0067(5) 1.3848(5) 0.9131(5) 0.0292(12) Uani 1 1 d . . . 
O29 O 0.1031(5) 0.6322(4) 0.6108(4) 0.0209(11) Uani 1 1 d . . . 
O30 O 0.0363(7) 0.6014(5) 0.4322(5) 0.0464(18) Uani 1 1 d . . . 
B1 B 0.8493(7) 1.2966(7) 1.0966(7) 0.0175(15) Uani 1 1 d . . . 
B2 B 0.9195(7) 1.3620(7) 0.9665(7) 0.0208(16) Uani 1 1 d . . . 
B3 B 0.6973(7) 1.2959(7) 0.9529(7) 0.0168(15) Uani 1 1 d . . . 
B4 B 0.4879(7) 1.2886(7) 0.9394(6) 0.0162(15) Uani 1 1 d . . . 
B5 B 0.2998(7) 1.3232(7) 0.9002(7) 0.0178(15) Uani 1 1 d . . . 
B6 B 0.2798(7) 1.1105(7) 0.8281(6) 0.0167(15) Uani 1 1 d . . . 
B7 B 0.2265(7) 0.8888(7) 0.6975(6) 0.0158(15) Uani 1 1 d . . . 
B8 B 0.1008(8) 0.6787(7) 0.5422(7) 0.0216(17) Uani 1 1 d . . . 
B9 B 0.1695(7) 0.7106(7) 0.7315(6) 0.0157(15) Uani 1 1 d . . . 
O1W O 0.5000 1.0000 1.0000 0.149(8) Uani 1 2 d S . . 
O2W O 1.0358(10) 0.0677(10) 0.3498(9) 0.043(3) Uiso 0.60 1 d P . . 
O2W' O 1.165(4) 0.165(4) 0.284(3) 0.079(16) Uiso 0.40 1 d P . . 
O3W O 0.3395(15) 0.1278(15) 0.4363(14) 0.142(5) Uiso 1 1 d . . . 
O4W O 0.3889(18) 0.2412(12) 0.6645(11) 0.067(5) Uani 0.50 1 d P . . 
O5W O 0.757(3) 0.408(3) 0.762(2) 0.118(8) Uiso 0.50 1 d P . . 
O6W O 1.1390(8) 0.3854(10) 0.2878(8) 0.094(4) Uani 1 1 d . . . 
O7W O -0.1766(7) -0.1837(10) -0.2651(7) 0.0307(18) Uani 1 1 d . . . 
O8W O -0.3927(18) -0.3871(18) -0.3953(16) 0.095(5) Uiso 0.60 1 d P . . 
O8W' O -0.468(3) -0.506(2) -0.375(2) 0.088(7) Uiso 0.40 1 d P . . 
O9W O 0.833(3) 0.195(2) 0.680(2) 0.080(9) Uani 0.50 1 d P . . 
O9W' O 0.852(3) 0.151(2) 0.653(2) 0.079(8) Uani 0.50 1 d P . . 
O10A O 0.1972(19) 0.9992(18) 0.5221(16) 0.093(5) Uiso 0.60 1 d P . . 
O10B O 0.105(3) 0.961(3) 0.517(3) 0.103(9) Uiso 0.40 1 d P . . 
O11B O 0.171(2) 0.273(2) 0.551(2) 0.118(7) Uiso 0.60 1 d P . . 
O11A O 0.102(3) 0.189(3) 0.647(3) 0.107(9) Uiso 0.40 1 d P . . 
O12W O 1.0119(14) 0.1473(18) 0.6938(12) 0.074(5) Uani 0.50 1 d P . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
V1 O18 1.618(5) . ? 
V1 O13 1.929(5) . ? 
V1 O15 1.933(5) . ? 
V1 O16 1.945(5) . ? 
V1 O12 1.957(5) . ? 
V1 V6 3.015(4) . ? 
V1 V2 3.017(3) . ? 
V1 K5 3.621(5) . ? 
V1 K3 3.736(5) 2_666 ? 
V2 O3 1.614(5) . ? 
V2 O6 1.925(5) . ? 
V2 O12 1.927(5) . ? 
V2 O15 1.952(5) . ? 
V2 O10 2.015(5) . ? 
V2 V3 2.988(3) . ? 
V2 K4 3.624(4) . ? 
V2 K5 3.730(6) . ? 
V2 K2 3.732(4) . ? 
V3 O1 1.617(5) . ? 
V3 O17 1.925(5) . ? 
V3 O15 1.926(5) . ? 
V3 O6 1.942(5) . ? 
V3 O14 1.950(5) 2_677 ? 
V3 V4 3.006(3) . ? 
V3 K1 3.538(4) . ? 
V3 K2 3.698(5) . ? 
V4 O4 1.610(5) . ? 
V4 O11 1.919(5) . ? 
V4 O14 1.933(5) 2_677 ? 
V4 O17 1.967(5) . ? 
V4 O7 1.986(5) 2_677 ? 
V4 V5 3.019(3) . ? 
V4 K1 3.537(4) . ? 
V4 K1 3.586(3) 2_777 ? 
V5 O2 1.627(5) . ? 
V5 O17 1.921(5) . ? 
V5 O13 1.930(5) . ? 
V5 O9 1.938(5) . ? 
V5 O11 1.946(5) . ? 
V5 V6 2.985(3) . ? 
V5 K1 3.577(4) 2_777 ? 
V6 O5 1.619(5) . ? 
V6 O9 1.916(5) . ? 
V6 O16 1.938(5) . ? 
V6 O13 1.957(5) . ? 
V6 O8 2.010(5) . ? 
V6 K3 3.680(5) 2_666 ? 
K1 O2 2.759(6) 2_777 ? 
K1 O1 2.772(6) . ? 
K1 O4 2.847(6) . ? 
K1 O4 2.864(6) 2_777 ? 
K1 O24 2.866(6) 2_777 ? 
K1 O19 2.927(6) 2_677 ? 
K1 O14 3.077(6) 2_677 ? 
K1 O11 3.142(6) 2_777 ? 
K1 B2 3.376(8) 2_777 ? 
K1 O28 3.420(6) 2_777 ? 
K1 B5 3.488(9) 2_677 ? 
K2 O4W 2.736(15) . ? 
K2 O27 2.830(6) 1_545 ? 
K2 O27 2.835(6) 2_677 ? 
K2 O25 2.886(5) 1_545 ? 
K2 O1 2.893(6) . ? 
K2 O5W 2.93(3) . ? 
K2 O3 2.998(6) . ? 
K2 O8W' 3.02(3) 1_666 ? 
K2 O6 3.243(6) . ? 
K2 B5 3.338(9) 2_677 ? 
K2 O26 3.346(7) 2_677 ? 
K2 B4 3.367(8) 1_545 ? 
K3 O9W 2.61(3) . ? 
K3 O5 2.872(6) 1_545 ? 
K3 O5 2.901(7) 2_666 ? 
K3 O9W' 2.91(3) . ? 
K3 O18 2.949(7) 2_666 ? 
K3 O5W 2.96(3) . ? 
K3 O21 3.018(7) 2_666 ? 
K3 O16 3.237(7) 2_666 ? 
K3 O10A 3.26(2) 2_666 ? 
K3 V6 3.680(5) 2_666 ? 
K3 V1 3.736(5) 2_666 ? 
K3 K3 4.508(8) 2_656 ? 
K4 O30 2.668(6) 2_566 ? 
K4 O28 2.675(6) 1_445 ? 
K4 O11A 2.77(3) . ? 
K4 O3 2.928(7) . ? 
K4 O26 2.977(6) 1_545 ? 
K4 O23 2.988(6) . ? 
K4 O10 3.036(5) . ? 
K4 O12W 3.08(2) 1_455 ? 
K4 O11B 3.09(2) . ? 
K4 O9W 3.13(3) 1_455 ? 
K4 B1 3.232(9) 2_677 ? 
K4 O24 3.237(6) 2_677 ? 
K5 O11B 2.81(2) . ? 
K5 O18 2.814(7) . ? 
K5 O8W 2.82(2) 2 ? 
K5 O6W 2.853(12) 1_455 ? 
K5 O29 2.947(7) . ? 
K5 O3 3.044(8) . ? 
K5 O12 3.165(7) . ? 
K5 O30 3.352(10) 2_566 ? 
K5 B8 3.499(10) . ? 
O2 K1 2.759(6) 2_777 ? 
O4 K1 2.864(6) 2_777 ? 
O5 K3 2.872(6) 1_565 ? 
O5 K3 2.901(7) 2_666 ? 
O6 B4 1.487(9) 2_677 ? 
O7 B9 1.505(9) . ? 
O7 B7 1.519(9) . ? 
O7 V4 1.986(5) 2_677 ? 
O8 B4 1.516(9) . ? 
O8 B6 1.517(9) . ? 
O9 B3 1.466(9) . ? 
O10 B1 1.511(9) 2_677 ? 
O10 B3 1.527(9) 2_677 ? 
O11 B1 1.468(9) . ? 
O11 K1 3.142(6) 2_777 ? 
O12 B9 1.467(9) . ? 
O14 B6 1.470(9) . ? 
O14 V4 1.933(5) 2_677 ? 
O14 V3 1.950(5) 2_677 ? 
O14 K1 3.077(6) 2_677 ? 
O16 B7 1.464(9) . ? 
O16 K3 3.237(7) 2_666 ? 
O18 K3 2.949(7) 2_666 ? 
O19 B5 1.360(9) . ? 
O19 B6 1.491(9) . ? 
O19 K1 2.927(6) 2_677 ? 
O20 B6 1.427(9) . ? 
O20 B7 1.431(9) . ? 
O21 B8 1.346(10) . ? 
O21 B7 1.473(9) . ? 
O21 K3 3.018(7) 2_666 ? 
O22 B2 1.352(10) . ? 
O22 B3 1.482(9) . ? 
O23 B1 1.416(9) 2_677 ? 
O23 B9 1.442(9) . ? 
O24 B2 1.357(10) . ? 
O24 B1 1.494(9) . ? 
O24 K1 2.866(6) 2_777 ? 
O24 K4 3.237(6) 2_677 ? 
O25 B3 1.427(9) . ? 
O25 B4 1.434(9) . ? 
O25 K2 2.886(5) 1_565 ? 
O26 B5 1.380(9) . ? 
O26 K4 2.977(6) 1_565 ? 
O26 K2 3.346(7) 2_677 ? 
O27 B5 1.349(9) . ? 
O27 B4 1.460(9) . ? 
O27 K2 2.830(6) 1_565 ? 
O27 K2 2.835(6) 2_677 ? 
O28 B2 1.384(10) . ? 
O28 K4 2.675(6) 1_665 ? 
O28 K1 3.420(6) 2_777 ? 
O29 B8 1.363(10) . ? 
O29 B9 1.474(9) . ? 
O30 B8 1.357(10) . ? 
O30 K4 2.668(6) 2_566 ? 
O30 K5 3.352(10) 2_566 ? 
B1 O23 1.416(9) 2_677 ? 
B1 O10 1.511(9) 2_677 ? 
B1 K4 3.232(9) 2_677 ? 
B1 K1 3.554(8) 2_777 ? 
B2 K1 3.376(8) 2_777 ? 
B3 O10 1.527(9) 2_677 ? 
B4 O6 1.487(9) 2_677 ? 
B4 K2 3.367(8) 1_565 ? 
B4 K2 3.577(8) 2_677 ? 
B5 K2 3.338(9) 2_677 ? 
B5 K1 3.488(8) 2_677 ? 
B5 K2 3.561(8) 1_565 ? 
B6 K1 3.559(9) 2_677 ? 
O6W K5 2.853(12) 1_655 ? 
O8W O8W' 1.73(3) . ? 
O8W K5 2.82(2) 2 ? 
O8W' K2 3.02(3) 1_444 ? 
O9W O9W' 0.66(3) . ? 
O9W K4 3.13(3) 1_655 ? 
O9W' K4 3.28(3) 1_655 ? 
O10A O10B 1.04(3) . ? 
O10A K3 3.26(2) 2_666 ? 
O11A O12W 1.43(4) 1_455 ? 
O12W O11A 1.43(4) 1_655 ? 
O12W K4 3.08(2) 1_655 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O18 V1 O13 106.8(3) . . ? 
O18 V1 O15 108.3(3) . . ? 
O13 V1 O15 93.8(2) . . ? 
O18 V1 O16 107.1(2) . . ? 
O13 V1 O16 78.4(2) . . ? 
O15 V1 O16 144.5(2) . . ? 
O18 V1 O12 107.3(3) . . ? 
O13 V1 O12 145.9(2) . . ? 
O15 V1 O12 77.9(2) . . ? 
O16 V1 O12 89.4(2) . . ? 
O18 V1 V6 110.5(2) . . ? 
O13 V1 V6 39.45(15) . . ? 
O15 V1 V6 125.88(16) . . ? 
O16 V1 V6 38.98(15) . . ? 
O12 V1 V6 122.62(15) . . ? 
O18 V1 V2 111.6(2) . . ? 
O13 V1 V2 126.30(16) . . ? 
O15 V1 V2 39.28(15) . . ? 
O16 V1 V2 121.85(16) . . ? 
O12 V1 V2 38.67(14) . . ? 
V6 V1 V2 137.86(6) . . ? 
O18 V1 K5 48.2(2) . . ? 
O13 V1 K5 152.69(17) . . ? 
O15 V1 K5 86.37(18) . . ? 
O16 V1 K5 116.14(18) . . ? 
O12 V1 K5 60.74(17) . . ? 
V6 V1 K5 147.67(10) . . ? 
V2 V1 K5 67.66(11) . . ? 
O18 V1 K3 49.3(2) . 2_666 ? 
O13 V1 K3 83.42(16) . 2_666 ? 
O15 V1 K3 154.24(16) . 2_666 ? 
O16 V1 K3 60.02(16) . 2_666 ? 
O12 V1 K3 117.82(16) . 2_666 ? 
V6 V1 K3 65.03(7) . 2_666 ? 
V2 V1 K3 150.23(7) . 2_666 ? 
K5 V1 K3 84.76(12) . 2_666 ? 
O3 V2 O6 109.7(2) . . ? 
O3 V2 O12 108.8(3) . . ? 
O6 V2 O12 139.6(2) . . ? 
O3 V2 O15 107.9(3) . . ? 
O6 V2 O15 78.7(2) . . ? 
O12 V2 O15 78.2(2) . . ? 
O3 V2 O10 104.8(2) . . ? 
O6 V2 O10 90.2(2) . . ? 
O12 V2 O10 91.7(2) . . ? 
O15 V2 O10 147.3(2) . . ? 
O3 V2 V3 112.0(2) . . ? 
O6 V2 V3 39.60(15) . . ? 
O12 V2 V3 112.41(16) . . ? 
O15 V2 V3 39.28(15) . . ? 
O10 V2 V3 124.85(15) . . ? 
O3 V2 V1 112.3(2) . . ? 
O6 V2 V1 112.05(16) . . ? 
O12 V2 V1 39.39(15) . . ? 
O15 V2 V1 38.82(14) . . ? 
O10 V2 V1 125.32(14) . . ? 
V3 V2 V1 75.58(6) . . ? 
O3 V2 K4 52.2(2) . . ? 
O6 V2 K4 124.35(16) . . ? 
O12 V2 K4 89.43(17) . . ? 
O15 V2 K4 151.75(16) . . ? 
O10 V2 K4 56.90(14) . . ? 
V3 V2 K4 157.41(6) . . ? 
V1 V2 K4 123.55(7) . . ? 
O3 V2 K5 53.0(2) . . ? 
O6 V2 K5 148.92(17) . . ? 
O12 V2 K5 58.05(17) . . ? 
O15 V2 K5 83.07(17) . . ? 
O10 V2 K5 117.82(17) . . ? 
V3 V2 K5 117.02(8) . . ? 
V1 V2 K5 63.91(10) . . ? 
K4 V2 K5 68.90(8) . . ? 
O3 V2 K2 51.2(2) . . ? 
O6 V2 K2 60.32(16) . . ? 
O12 V2 K2 148.20(16) . . ? 
O15 V2 K2 85.22(16) . . ? 
O10 V2 K2 115.92(14) . . ? 
V3 V2 K2 65.70(9) . . ? 
V1 V2 K2 118.53(7) . . ? 
K4 V2 K2 92.81(11) . . ? 
K5 V2 K2 93.39(9) . . ? 
O1 V3 O17 107.8(3) . . ? 
O1 V3 O15 107.1(3) . . ? 
O17 V3 O15 93.7(2) . . ? 
O1 V3 O6 108.2(3) . . ? 
O17 V3 O6 143.9(2) . . ? 
O15 V3 O6 79.0(2) . . ? 
O1 V3 O14 106.7(2) . 2_677 ? 
O17 V3 O14 79.0(2) . 2_677 ? 
O15 V3 O14 146.1(2) . 2_677 ? 
O6 V3 O14 87.7(2) . 2_677 ? 
O1 V3 V2 110.5(2) . . ? 
O17 V3 V2 126.45(15) . . ? 
O15 V3 V2 39.92(15) . . ? 
O6 V3 V2 39.19(15) . . ? 
O14 V3 V2 122.02(15) 2_677 . ? 
O1 V3 V4 111.1(2) . . ? 
O17 V3 V4 39.93(15) . . ? 
O15 V3 V4 126.65(16) . . ? 
O6 V3 V4 120.45(16) . . ? 
O14 V3 V4 39.07(14) 2_677 . ? 
V2 V3 V4 138.15(5) . . ? 
O1 V3 K1 49.4(2) . . ? 
O17 V3 K1 82.94(16) . . ? 
O15 V3 K1 152.39(16) . . ? 
O6 V3 K1 119.01(16) . . ? 
O14 V3 K1 60.23(15) 2_677 . ? 
V2 V3 K1 150.51(7) . . ? 
V4 V3 K1 64.84(7) . . ? 
O1 V3 K2 48.5(2) . . ? 
O17 V3 K2 154.41(16) . . ? 
O15 V3 K2 86.53(15) . . ? 
O6 V3 K2 61.15(15) . . ? 
O14 V3 K2 114.12(15) 2_677 . ? 
V2 V3 K2 66.88(5) . . ? 
V4 V3 K2 146.81(6) . . ? 
K1 V3 K2 85.15(6) . . ? 
O4 V4 O11 109.0(2) . . ? 
O4 V4 O14 109.1(2) . 2_677 ? 
O11 V4 O14 139.8(2) . 2_677 ? 
O4 V4 O17 109.4(2) . . ? 
O11 V4 O17 77.4(2) . . ? 
O14 V4 O17 78.4(2) 2_677 . ? 
O4 V4 O7 103.5(2) . 2_677 ? 
O11 V4 O7 91.4(2) . 2_677 ? 
O14 V4 O7 91.9(2) 2_677 2_677 ? 
O17 V4 O7 147.1(2) . 2_677 ? 
O4 V4 V3 113.7(2) . . ? 
O11 V4 V3 111.16(17) . . ? 
O14 V4 V3 39.48(15) 2_677 . ? 
O17 V4 V3 38.92(14) . . ? 
O7 V4 V3 125.37(15) 2_677 . ? 
O4 V4 V5 113.0(2) . . ? 
O11 V4 V5 38.97(14) . . ? 
O14 V4 V5 111.99(15) 2_677 . ? 
O17 V4 V5 38.52(15) . . ? 
O7 V4 V5 125.00(15) 2_677 . ? 
V3 V4 V5 74.93(7) . . ? 
O4 V4 K1 52.10(19) . . ? 
O11 V4 K1 145.04(16) . . ? 
O14 V4 K1 60.28(17) 2_677 . ? 
O17 V4 K1 82.43(15) . . ? 
O7 V4 K1 119.91(14) 2_677 . ? 
V3 V4 K1 64.87(9) . . ? 
V5 V4 K1 114.92(6) . . ? 
O4 V4 K1 51.1(2) . 2_777 ? 
O11 V4 K1 61.02(16) . 2_777 ? 
O14 V4 K1 144.85(16) 2_677 2_777 ? 
O17 V4 K1 82.36(17) . 2_777 ? 
O7 V4 K1 119.24(15) 2_677 2_777 ? 
V3 V4 K1 115.19(8) . 2_777 ? 
V5 V4 K1 64.92(8) . 2_777 ? 
K1 V4 K1 88.36(8) . 2_777 ? 
O2 V5 O17 106.8(2) . . ? 
O2 V5 O13 107.3(3) . . ? 
O17 V5 O13 94.3(2) . . ? 
O2 V5 O9 110.3(2) . . ? 
O17 V5 O9 142.6(2) . . ? 
O13 V5 O9 78.9(2) . . ? 
O2 V5 O11 106.5(3) . . ? 
O17 V5 O11 77.8(2) . . ? 
O13 V5 O11 146.1(2) . . ? 
O9 V5 O11 87.6(2) . . ? 
O2 V5 V6 111.3(2) . . ? 
O17 V5 V6 127.14(16) . . ? 
O13 V5 V6 40.17(15) . . ? 
O9 V5 V6 38.98(14) . . ? 
O11 V5 V6 122.20(15) . . ? 
O2 V5 V4 109.7(2) . . ? 
O17 V5 V4 39.60(15) . . ? 
O13 V5 V4 127.32(16) . . ? 
O9 V5 V4 119.70(15) . . ? 
O11 V5 V4 38.31(15) . . ? 
V6 V5 V4 138.81(5) . . ? 
O2 V5 K1 47.7(2) . 2_777 ? 
O17 V5 K1 83.17(16) . 2_777 ? 
O13 V5 K1 151.48(15) . 2_777 ? 
O9 V5 K1 119.46(16) . 2_777 ? 
O11 V5 K1 61.20(15) . 2_777 ? 
V6 V5 K1 149.54(6) . 2_777 ? 
V4 V5 K1 65.23(5) . 2_777 ? 
O5 V6 O9 112.7(3) . . ? 
O5 V6 O16 109.1(3) . . ? 
O9 V6 O16 136.5(2) . . ? 
O5 V6 O13 107.1(3) . . ? 
O9 V6 O13 78.8(2) . . ? 
O16 V6 O13 77.9(2) . . ? 
O5 V6 O8 106.4(2) . . ? 
O9 V6 O8 88.8(2) . . ? 
O16 V6 O8 90.9(2) . . ? 
O13 V6 O8 146.5(2) . . ? 
O5 V6 V5 112.7(2) . . ? 
O9 V6 V5 39.52(15) . . ? 
O16 V6 V5 111.57(16) . . ? 
O13 V6 V5 39.51(14) . . ? 
O8 V6 V5 123.78(15) . . ? 
O5 V6 V1 111.9(2) . . ? 
O9 V6 V1 110.82(15) . . ? 
O16 V6 V1 39.14(14) . . ? 
O13 V6 V1 38.78(15) . . ? 
O8 V6 V1 124.24(15) . . ? 
V5 V6 V1 75.35(5) . . ? 
O5 V6 K3 49.4(2) . 2_666 ? 
O9 V6 K3 150.18(17) . 2_666 ? 
O16 V6 K3 61.44(16) . 2_666 ? 
O13 V6 K3 84.66(16) . 2_666 ? 
O8 V6 K3 117.65(16) . 2_666 ? 
V5 V6 K3 118.37(9) . 2_666 ? 
V1 V6 K3 66.99(8) . 2_666 ? 
O2 K1 O1 175.67(17) 2_777 . ? 
O2 K1 O4 86.00(16) 2_777 . ? 
O1 K1 O4 97.89(15) . . ? 
O2 K1 O4 96.50(17) 2_777 2_777 ? 
O1 K1 O4 87.16(17) . 2_777 ? 
O4 K1 O4 59.25(19) . 2_777 ? 
O2 K1 O24 76.38(17) 2_777 2_777 ? 
O1 K1 O24 101.20(17) . 2_777 ? 
O4 K1 O24 145.02(16) . 2_777 ? 
O4 K1 O24 92.63(16) 2_777 2_777 ? 
O2 K1 O19 100.59(17) 2_777 2_677 ? 
O1 K1 O19 77.34(17) . 2_677 ? 
O4 K1 O19 93.51(15) . 2_677 ? 
O4 K1 O19 146.65(15) 2_777 2_677 ? 
O24 K1 O19 119.09(15) 2_777 2_677 ? 
O2 K1 O14 122.84(17) 2_777 2_677 ? 
O1 K1 O14 58.47(15) . 2_677 ? 
O4 K1 O14 58.31(14) . 2_677 ? 
O4 K1 O14 99.88(15) 2_777 2_677 ? 
O24 K1 O14 155.12(15) 2_777 2_677 ? 
O19 K1 O14 46.90(13) 2_677 2_677 ? 
O2 K1 O11 57.77(16) 2_777 2_777 ? 
O1 K1 O11 123.15(17) . 2_777 ? 
O4 K1 O11 98.31(14) . 2_777 ? 
O4 K1 O11 57.05(14) 2_777 2_777 ? 
O24 K1 O11 46.76(13) 2_777 2_777 ? 
O19 K1 O11 154.18(14) 2_677 2_777 ? 
O14 K1 O11 154.97(14) 2_677 2_777 ? 
O2 K1 B2 62.81(19) 2_777 2_777 ? 
O1 K1 B2 113.7(2) . 2_777 ? 
O4 K1 B2 147.31(19) . 2_777 ? 
O4 K1 B2 112.03(19) 2_777 2_777 ? 
O24 K1 B2 23.32(18) 2_777 2_777 ? 
O19 K1 B2 101.25(18) 2_677 2_777 ? 
O14 K1 B2 147.08(18) 2_677 2_777 ? 
O11 K1 B2 57.83(17) 2_777 2_777 ? 
O2 K1 O28 69.52(16) 2_777 2_777 ? 
O1 K1 O28 106.23(16) . 2_777 ? 
O4 K1 O28 151.67(17) . 2_777 ? 
O4 K1 O28 135.28(15) 2_777 2_777 ? 
O24 K1 O28 43.42(14) 2_777 2_777 ? 
O19 K1 O28 77.85(14) 2_677 2_777 ? 
O14 K1 O28 123.73(14) 2_677 2_777 ? 
O11 K1 O28 80.93(13) 2_777 2_777 ? 
B2 K1 O28 23.49(17) 2_777 2_777 ? 
O2 K1 B5 112.53(19) 2_777 2_677 ? 
O1 K1 B5 64.25(19) . 2_677 ? 
O4 K1 B5 112.40(18) . 2_677 ? 
O4 K1 B5 149.66(18) 2_777 2_677 ? 
O24 K1 B5 102.28(19) 2_777 2_677 ? 
O19 K1 B5 22.36(16) 2_677 2_677 ? 
O14 K1 B5 57.45(17) 2_677 2_677 ? 
O11 K1 B5 147.57(17) 2_777 2_677 ? 
B2 K1 B5 89.9(2) 2_777 2_677 ? 
O28 K1 B5 67.15(17) 2_777 2_677 ? 
O2 K1 V4 108.20(14) 2_777 . ? 
O1 K1 V4 75.10(12) . . ? 
O4 K1 V4 26.51(11) . . ? 
O4 K1 V4 71.97(12) 2_777 . ? 
O24 K1 V4 164.18(12) 2_777 . ? 
O19 K1 V4 75.56(11) 2_677 . ? 
O14 K1 V4 33.07(9) 2_677 . ? 
O11 K1 V4 122.21(11) 2_777 . ? 
B2 K1 V4 170.07(16) 2_777 . ? 
O28 K1 V4 152.36(12) 2_777 . ? 
B5 K1 V4 90.06(15) 2_677 . ? 
O4W K2 O27 74.8(4) . 1_545 ? 
O4W K2 O27 136.3(4) . 2_677 ? 
O27 K2 O27 63.58(18) 1_545 2_677 ? 
O4W K2 O25 84.5(3) . 1_545 ? 
O27 K2 O25 48.23(14) 1_545 1_545 ? 
O27 K2 O25 77.95(16) 2_677 1_545 ? 
O4W K2 O1 143.8(4) . . ? 
O27 K2 O1 139.99(16) 1_545 . ? 
O27 K2 O1 76.42(16) 2_677 . ? 
O25 K2 O1 124.16(17) 1_545 . ? 
O4W K2 O5W 90.2(7) . . ? 
O27 K2 O5W 119.4(6) 1_545 . ? 
O27 K2 O5W 121.0(6) 2_677 . ? 
O25 K2 O5W 72.5(6) 1_545 . ? 
O1 K2 O5W 79.9(6) . . ? 
O4W K2 O3 76.5(4) . . ? 
O27 K2 O3 92.09(17) 1_545 . ? 
O27 K2 O3 91.70(16) 2_677 . ? 
O25 K2 O3 139.62(16) 1_545 . ? 
O1 K2 O3 89.83(17) . . ? 
O5W K2 O3 141.5(6) . . ? 
O4W K2 O8W' 77.9(6) . 1_666 ? 
O27 K2 O8W' 145.7(5) 1_545 1_666 ? 
O27 K2 O8W' 132.6(5) 2_677 1_666 ? 
O25 K2 O8W' 147.7(5) 1_545 1_666 ? 
O1 K2 O8W' 66.2(5) . 1_666 ? 
O5W K2 O8W' 80.7(7) . 1_666 ? 
O3 K2 O8W' 61.3(5) . 1_666 ? 
O4W K2 O6 130.1(4) . . ? 
O27 K2 O6 93.72(15) 1_545 . ? 
O27 K2 O6 45.78(13) 2_677 . ? 
O25 K2 O6 123.54(16) 1_545 . ? 
O1 K2 O6 55.80(15) . . ? 
O5W K2 O6 134.8(6) . . ? 
O3 K2 O6 55.17(13) . . ? 
O8W' K2 O6 88.2(5) 1_666 . ? 
O4W K2 B5 150.9(4) . 2_677 ? 
O27 K2 B5 76.89(19) 1_545 2_677 ? 
O27 K2 B5 23.47(17) 2_677 2_677 ? 
O25 K2 B5 71.61(19) 1_545 2_677 ? 
O1 K2 B5 65.32(18) . 2_677 ? 
O5W K2 B5 97.8(6) . 2_677 ? 
O3 K2 B5 111.39(18) . 2_677 ? 
O8W' K2 B5 130.9(5) 1_666 2_677 ? 
O6 K2 B5 58.32(16) . 2_677 ? 
O4W K2 O26 137.1(3) . 2_677 ? 
O27 K2 O26 75.59(16) 1_545 2_677 ? 
O27 K2 O26 43.73(14) 2_677 2_677 ? 
O25 K2 O26 52.66(14) 1_545 2_677 ? 
O1 K2 O26 74.98(15) . 2_677 ? 
O5W K2 O26 78.1(6) . 2_677 ? 
O3 K2 O26 134.85(15) . 2_677 ? 
O8W' K2 O26 138.4(5) 1_666 2_677 ? 
O6 K2 O26 82.02(13) . 2_677 ? 
B5 K2 O26 23.84(16) 2_677 2_677 ? 
O4W K2 B4 71.3(3) . 1_545 ? 
O27 K2 B4 25.42(16) 1_545 1_545 ? 
O27 K2 B4 76.33(19) 2_677 1_545 ? 
O25 K2 B4 25.02(16) 1_545 1_545 ? 
O1 K2 B4 143.57(18) . 1_545 ? 
O5W K2 B4 94.0(6) . 1_545 ? 
O3 K2 B4 114.66(19) . 1_545 ? 
O8W' K2 B4 148.7(5) 1_666 1_545 ? 
O6 K2 B4 115.71(18) . 1_545 ? 
B5 K2 B4 80.3(2) 2_677 1_545 ? 
O26 K2 B4 68.63(17) 2_677 1_545 ? 
O9W K3 O5 81.6(8) . 1_545 ? 
O9W K3 O5 119.0(5) . 2_666 ? 
O5 K3 O5 77.3(2) 1_545 2_666 ? 
O9W K3 O9W' 12.4(6) . . ? 
O5 K3 O9W' 83.7(6) 1_545 . ? 
O5 K3 O9W' 108.0(5) 2_666 . ? 
O9W K3 O18 141.2(7) . 2_666 ? 
O5 K3 O18 131.6(2) 1_545 2_666 ? 
O5 K3 O18 91.38(19) 2_666 2_666 ? 
O9W' K3 O18 143.5(6) . 2_666 ? 
O9W K3 O5W 64.9(7) . . ? 
O5 K3 O5W 88.8(6) 1_545 . ? 
O5 K3 O5W 164.3(6) 2_666 . ? 
O9W' K3 O5W 77.1(7) . . ? 
O18 K3 O5W 92.6(6) 2_666 . ? 
O9W K3 O21 80.9(8) . 2_666 ? 
O5 K3 O21 151.8(2) 1_545 2_666 ? 
O5 K3 O21 92.10(18) 2_666 2_666 ? 
O9W' K3 O21 74.8(6) . 2_666 ? 
O18 K3 O21 73.90(17) 2_666 2_666 ? 
O5W K3 O21 103.6(6) . 2_666 ? 
O9W K3 O16 120.9(8) . 2_666 ? 
O5 K3 O16 133.38(19) 1_545 2_666 ? 
O5 K3 O16 56.14(15) 2_666 2_666 ? 
O9W' K3 O16 110.8(5) . 2_666 ? 
O18 K3 O16 55.11(15) 2_666 2_666 ? 
O5W K3 O16 136.9(6) . 2_666 ? 
O21 K3 O16 45.01(13) 2_666 2_666 ? 
O9W K3 O10A 53.8(7) . 2_666 ? 
O5 K3 O10A 93.8(4) 1_545 2_666 ? 
O5 K3 O10A 71.3(4) 2_666 2_666 ? 
O9W' K3 O10A 41.4(6) . 2_666 ? 
O18 K3 O10A 127.2(4) 2_666 2_666 ? 
O5W K3 O10A 117.4(7) . 2_666 ? 
O21 K3 O10A 58.1(4) 2_666 2_666 ? 
O16 K3 O10A 74.8(4) 2_666 2_666 ? 
O9W K3 V6 128.8(6) . 2_666 ? 
O5 K3 V6 101.75(17) 1_545 2_666 ? 
O5 K3 V6 25.09(11) 2_666 2_666 ? 
O9W' K3 V6 116.4(5) . 2_666 ? 
O18 K3 V6 70.86(14) 2_666 2_666 ? 
O5W K3 V6 163.5(5) . 2_666 ? 
O21 K3 V6 72.92(13) 2_666 2_666 ? 
O16 K3 V6 31.73(10) 2_666 2_666 ? 
O10A K3 V6 75.0(4) 2_666 2_666 ? 
O9W K3 V1 142.7(8) . 2_666 ? 
O5 K3 V1 134.40(17) 1_545 2_666 ? 
O5 K3 V1 71.11(14) 2_666 2_666 ? 
O9W' K3 V1 136.9(6) . 2_666 ? 
O18 K3 V1 24.59(10) 2_666 2_666 ? 
O5W K3 V1 115.8(5) . 2_666 ? 
O21 K3 V1 62.33(12) 2_666 2_666 ? 
O16 K3 V1 31.36(10) 2_666 2_666 ? 
O10A K3 V1 105.9(4) 2_666 2_666 ? 
V6 K3 V1 47.97(8) 2_666 2_666 ? 
O9W K3 K3 102.7(6) . 2_656 ? 
O5 K3 K3 38.88(13) 1_545 2_656 ? 
O5 K3 K3 38.42(13) 2_666 2_656 ? 
O9W' K3 K3 97.4(6) . 2_656 ? 
O18 K3 K3 115.98(18) 2_666 2_656 ? 
O5W K3 K3 127.3(6) . 2_656 ? 
O21 K3 K3 125.80(18) 2_666 2_656 ? 
O16 K3 K3 94.53(14) 2_666 2_656 ? 
O10A K3 K3 80.5(4) 2_666 2_656 ? 
V6 K3 K3 63.06(9) 2_666 2_656 ? 
V1 K3 K3 103.73(12) 2_666 2_656 ? 
O30 K4 O28 132.7(2) 2_566 1_445 ? 
O30 K4 O11A 98.3(7) 2_566 . ? 
O28 K4 O11A 93.9(7) 1_445 . ? 
O30 K4 O3 100.0(2) 2_566 . ? 
O28 K4 O3 126.66(17) 1_445 . ? 
O11A K4 O3 85.0(7) . . ? 
O30 K4 O26 167.5(2) 2_566 1_545 ? 
O28 K4 O26 57.67(17) 1_445 1_545 ? 
O11A K4 O26 72.3(7) . 1_545 ? 
O3 K4 O26 71.57(17) . 1_545 ? 
O30 K4 O23 67.50(16) 2_566 . ? 
O28 K4 O23 109.52(17) 1_445 . ? 
O11A K4 O23 156.6(7) . . ? 
O3 K4 O23 79.64(15) . . ? 
O26 K4 O23 118.35(15) 1_545 . ? 
O30 K4 O10 112.75(17) 2_566 . ? 
O28 K4 O10 89.19(18) 1_445 . ? 
O11A K4 O10 134.1(7) . . ? 
O3 K4 O10 57.83(14) . . ? 
O26 K4 O10 71.04(15) 1_545 . ? 
O23 K4 O10 47.59(14) . . ? 
O30 K4 O12W 105.6(3) 2_566 1_455 ? 
O28 K4 O12W 69.2(4) 1_445 1_455 ? 
O11A K4 O12W 27.6(7) . 1_455 ? 
O3 K4 O12W 109.4(4) . 1_455 ? 
O26 K4 O12W 69.9(3) 1_545 1_455 ? 
O23 K4 O12W 169.9(3) . 1_455 ? 
O10 K4 O12W 141.0(3) . 1_455 ? 
O30 K4 O11B 70.7(5) 2_566 . ? 
O28 K4 O11B 137.1(5) 1_445 . ? 
O11A K4 O11B 43.4(8) . . ? 
O3 K4 O11B 59.2(4) . . ? 
O26 K4 O11B 96.9(5) 1_545 . ? 
O23 K4 O11B 113.1(4) . . ? 
O10 K4 O11B 116.4(5) . . ? 
O12W K4 O11B 69.6(6) 1_455 . ? 
O30 K4 O9W 80.4(5) 2_566 1_455 ? 
O28 K4 O9W 62.4(5) 1_445 1_455 ? 
O11A K4 O9W 67.8(9) . 1_455 ? 
O3 K4 O9W 152.4(5) . 1_455 ? 
O26 K4 O9W 102.8(5) 1_545 1_455 ? 
O23 K4 O9W 124.4(5) . 1_455 ? 
O10 K4 O9W 147.4(5) . 1_455 ? 
O12W K4 O9W 45.7(6) 1_455 1_455 ? 
O11B K4 O9W 95.9(7) . 1_455 ? 
O30 K4 B1 93.0(2) 2_566 2_677 ? 
O28 K4 B1 89.0(2) 1_445 2_677 ? 
O11A K4 B1 161.6(7) . 2_677 ? 
O3 K4 B1 78.81(18) . 2_677 ? 
O26 K4 B1 94.22(18) 1_545 2_677 ? 
O23 K4 B1 25.94(17) . 2_677 ? 
O10 K4 B1 27.66(16) . 2_677 ? 
O12W K4 B1 157.6(3) 1_455 2_677 ? 
O11B K4 B1 129.8(5) . 2_677 ? 
O9W K4 B1 128.7(6) 1_455 2_677 ? 
O30 K4 O24 99.9(2) 2_566 2_677 ? 
O28 K4 O24 65.35(17) 1_445 2_677 ? 
O11A K4 O24 158.6(7) . 2_677 ? 
O3 K4 O24 102.91(15) . 2_677 ? 
O26 K4 O24 91.06(16) 1_545 2_677 ? 
O23 K4 O24 44.30(14) . 2_677 ? 
O10 K4 O24 45.73(14) . 2_677 ? 
O12W K4 O24 134.0(4) 1_455 2_677 ? 
O11B K4 O24 156.2(4) . 2_677 ? 
O9W K4 O24 104.2(6) 1_455 2_677 ? 
B1 K4 O24 26.70(17) 2_677 2_677 ? 
O11B K5 O18 149.5(5) . . ? 
O11B K5 O8W 90.3(6) . 2 ? 
O18 K5 O8W 82.9(4) . 2 ? 
O11B K5 O6W 108.1(6) . 1_455 ? 
O18 K5 O6W 97.2(3) . 1_455 ? 
O8W K5 O6W 69.0(4) 2 1_455 ? 
O11B K5 O29 113.6(5) . . ? 
O18 K5 O29 78.4(2) . . ? 
O8W K5 O29 155.7(4) 2 . ? 
O6W K5 O29 98.1(3) 1_455 . ? 
O11B K5 O3 60.9(5) . . ? 
O18 K5 O3 92.22(18) . . ? 
O8W K5 O3 105.3(4) 2 . ? 
O6W K5 O3 168.1(3) 1_455 . ? 
O29 K5 O3 90.89(18) . . ? 
O11B K5 O12 109.5(5) . . ? 
O18 K5 O12 57.36(16) . . ? 
O8W K5 O12 131.4(4) 2 . ? 
O6W K5 O12 136.4(3) 1_455 . ? 
O29 K5 O12 46.20(14) . . ? 
O3 K5 O12 55.31(16) . . ? 
O11B K5 O30 65.1(5) . 2_566 ? 
O18 K5 O30 130.3(2) . 2_566 ? 
O8W K5 O30 145.8(4) 2 2_566 ? 
O6W K5 O30 95.2(2) 1_455 2_566 ? 
O29 K5 O30 52.31(17) . 2_566 ? 
O3 K5 O30 84.06(19) . 2_566 ? 
O12 K5 O30 81.24(17) . 2_566 ? 
O11B K5 B8 132.4(5) . . ? 
O18 K5 B8 67.7(2) . . ? 
O8W K5 B8 133.9(5) 2 . ? 
O6W K5 B8 80.1(3) 1_455 . ? 
O29 K5 B8 22.38(18) . . ? 
O3 K5 B8 110.3(2) . . ? 
O12 K5 B8 58.18(18) . . ? 
O30 K5 B8 67.5(2) 2_566 . ? 
O11B K5 V1 132.4(5) . . ? 
O18 K5 V1 25.38(12) . . ? 
O8W K5 V1 102.3(4) 2 . ? 
O6W K5 V1 119.3(3) 1_455 . ? 
O29 K5 V1 65.20(14) . . ? 
O3 K5 V1 71.55(14) . . ? 
O12 K5 V1 32.64(10) . . ? 
O30 K5 V1 111.82(16) 2_566 . ? 
B8 K5 V1 64.01(17) . . ? 
O11B K5 V2 84.6(5) . . ? 
O18 K5 V2 71.90(14) . . ? 
O8W K5 V2 115.6(4) 2 . ? 
O6W K5 V2 166.8(3) 1_455 . ? 
O29 K5 V2 72.90(13) . . ? 
O3 K5 V2 25.04(11) . . ? 
O12 K5 V2 31.10(10) . . ? 
O30 K5 V2 86.81(15) 2_566 . ? 
B8 K5 V2 88.67(16) . . ? 
V1 K5 V2 48.43(6) . . ? 
O11B K5 K4 47.9(5) . . ? 
O18 K5 K4 122.81(17) . . ? 
O8W K5 K4 134.8(4) 2 . ? 
O6W K5 K4 132.2(3) 1_455 . ? 
O29 K5 K4 69.22(14) . . ? 
O3 K5 K4 44.69(14) . . ? 
O12 K5 K4 66.22(14) . . ? 
O30 K5 K4 39.80(11) 2_566 . ? 
B8 K5 K4 91.23(18) . . ? 
V1 K5 K4 97.43(12) . . ? 
V2 K5 K4 54.36(10) . . ? 
V3 O1 K1 104.3(2) . . ? 
V3 O1 K2 106.7(3) . . ? 
K1 O1 K2 119.63(19) . . ? 
V5 O2 K1 106.4(3) . 2_777 ? 
V2 O3 K4 102.0(2) . . ? 
V2 O3 K2 104.0(2) . . ? 
K4 O3 K2 128.1(2) . . ? 
V2 O3 K5 102.0(3) . . ? 
K4 O3 K5 88.31(17) . . ? 
K2 O3 K5 128.0(2) . . ? 
V4 O4 K1 101.4(2) . . ? 
V4 O4 K1 102.9(2) . 2_777 ? 
K1 O4 K1 120.75(19) . 2_777 ? 
V6 O5 K3 149.0(3) . 1_565 ? 
V6 O5 K3 105.5(3) . 2_666 ? 
K3 O5 K3 102.7(2) 1_565 2_666 ? 
B4 O6 V2 130.4(4) 2_677 . ? 
B4 O6 V3 128.3(4) 2_677 . ? 
V2 O6 V3 101.2(2) . . ? 
B4 O6 K2 90.4(4) 2_677 . ? 
V2 O6 K2 88.65(17) . . ? 
V3 O6 K2 87.23(18) . . ? 
B9 O7 B7 114.9(5) . . ? 
B9 O7 V4 121.1(4) . 2_677 ? 
B7 O7 V4 121.5(4) . 2_677 ? 
B4 O8 B6 114.2(5) . . ? 
B4 O8 V6 120.9(4) . . ? 
B6 O8 V6 121.4(4) . . ? 
B3 O9 V6 130.6(4) . . ? 
B3 O9 V5 127.0(4) . . ? 
V6 O9 V5 101.5(2) . . ? 
B1 O10 B3 113.9(5) 2_677 2_677 ? 
B1 O10 V2 121.1(4) 2_677 . ? 
B3 O10 V2 120.3(4) 2_677 . ? 
B1 O10 K4 83.4(4) 2_677 . ? 
B3 O10 K4 119.1(4) 2_677 . ? 
V2 O10 K4 89.34(17) . . ? 
B1 O11 V4 129.3(4) . . ? 
B1 O11 V5 127.9(4) . . ? 
V4 O11 V5 102.7(2) . . ? 
B1 O11 K1 93.7(4) . 2_777 ? 
V4 O11 K1 86.70(17) . 2_777 ? 
V5 O11 K1 85.93(18) . 2_777 ? 
B9 O12 V2 129.8(4) . . ? 
B9 O12 V1 128.1(4) . . ? 
V2 O12 V1 101.9(2) . . ? 
B9 O12 K5 95.0(4) . . ? 
V2 O12 K5 90.9(2) . . ? 
V1 O12 K5 86.6(2) . . ? 
V1 O13 V5 143.7(3) . . ? 
V1 O13 V6 101.8(2) . . ? 
V5 O13 V6 100.3(2) . . ? 
B6 O14 V4 129.3(4) . 2_677 ? 
B6 O14 V3 129.2(4) . 2_677 ? 
V4 O14 V3 101.4(2) 2_677 2_677 ? 
B6 O14 K1 96.6(4) . 2_677 ? 
V4 O14 K1 86.66(19) 2_677 2_677 ? 
V3 O14 K1 86.40(18) 2_677 2_677 ? 
V3 O15 V1 144.9(3) . . ? 
V3 O15 V2 100.8(2) . . ? 
V1 O15 V2 101.9(2) . . ? 
B7 O16 V6 130.6(4) . . ? 
B7 O16 V1 127.5(4) . . ? 
V6 O16 V1 101.9(2) . . ? 
B7 O16 K3 94.6(4) . 2_666 ? 
V6 O16 K3 86.83(18) . 2_666 ? 
V1 O16 K3 88.63(18) . 2_666 ? 
V5 O17 V3 144.7(3) . . ? 
V5 O17 V4 101.9(2) . . ? 
V3 O17 V4 101.2(2) . . ? 
V1 O18 K5 106.4(3) . . ? 
V1 O18 K3 106.1(3) . 2_666 ? 
K5 O18 K3 118.8(2) . 2_666 ? 
B5 O19 B6 119.8(5) . . ? 
B5 O19 K1 102.7(4) . 2_677 ? 
B6 O19 K1 102.4(4) . 2_677 ? 
B6 O20 B7 121.5(5) . . ? 
B8 O21 B7 121.8(6) . . ? 
B8 O21 K3 107.8(5) . 2_666 ? 
B7 O21 K3 103.8(4) . 2_666 ? 
B2 O22 B3 122.1(6) . . ? 
B1 O23 B9 120.4(5) 2_677 . ? 
B1 O23 K4 86.7(4) 2_677 . ? 
B9 O23 K4 121.3(4) . . ? 
B2 O24 B1 120.4(6) . . ? 
B2 O24 K1 99.9(4) . 2_777 ? 
B1 O24 K1 104.8(4) . 2_777 ? 
B2 O24 K4 100.4(4) . 2_677 ? 
B1 O24 K4 76.5(4) . 2_677 ? 
K1 O24 K4 155.28(19) 2_777 2_677 ? 
B3 O25 B4 117.7(5) . . ? 
B3 O25 K2 141.3(4) . 1_565 ? 
B4 O25 K2 96.6(4) . 1_565 ? 
B5 O26 K4 125.6(5) . 1_565 ? 
B5 O26 K2 77.8(4) . 2_677 ? 
K4 O26 K2 153.82(19) 1_565 2_677 ? 
B5 O27 B4 123.0(6) . . ? 
B5 O27 K2 112.0(4) . 1_565 ? 
B4 O27 K2 98.3(4) . 1_565 ? 
B5 O27 K2 99.7(4) . 2_677 ? 
B4 O27 K2 108.5(4) . 2_677 ? 
K2 O27 K2 116.42(18) 1_565 2_677 ? 
B2 O28 K4 153.7(5) . 1_665 ? 
B2 O28 K1 76.5(4) . 2_777 ? 
K4 O28 K1 120.2(2) 1_665 2_777 ? 
B8 O29 B9 121.9(6) . . ? 
B8 O29 K5 102.2(5) . . ? 
B9 O29 K5 104.1(4) . . ? 
B8 O30 K4 144.2(5) . 2_566 ? 
B8 O30 K5 94.9(5) . 2_566 ? 
K4 O30 K5 86.7(2) 2_566 2_566 ? 
O23 B1 O11 111.1(6) 2_677 . ? 
O23 B1 O24 108.3(6) 2_677 . ? 
O11 B1 O24 108.1(6) . . ? 
O23 B1 O10 112.3(6) 2_677 2_677 ? 
O11 B1 O10 108.1(5) . 2_677 ? 
O24 B1 O10 108.9(5) . 2_677 ? 
O23 B1 K4 67.3(3) 2_677 2_677 ? 
O11 B1 K4 175.0(5) . 2_677 ? 
O24 B1 K4 76.8(4) . 2_677 ? 
O10 B1 K4 68.9(3) 2_677 2_677 ? 
O23 B1 K1 104.4(4) 2_677 2_777 ? 
O11 B1 K1 61.9(3) . 2_777 ? 
O24 B1 K1 51.2(3) . 2_777 ? 
O10 B1 K1 142.8(4) 2_677 2_777 ? 
K4 B1 K1 122.9(2) 2_677 2_777 ? 
O22 B2 O24 122.7(7) . . ? 
O22 B2 O28 116.6(7) . . ? 
O24 B2 O28 120.6(7) . . ? 
O22 B2 K1 136.2(5) . 2_777 ? 
O24 B2 K1 56.7(4) . 2_777 ? 
O28 B2 K1 80.0(4) . 2_777 ? 
O25 B3 O9 111.6(6) . . ? 
O25 B3 O22 107.6(6) . . ? 
O9 B3 O22 109.0(6) . . ? 
O25 B3 O10 112.6(6) . 2_677 ? 
O9 B3 O10 107.9(5) . 2_677 ? 
O22 B3 O10 108.1(5) . 2_677 ? 
O25 B4 O27 107.7(5) . . ? 
O25 B4 O6 110.5(5) . 2_677 ? 
O27 B4 O6 108.6(6) . 2_677 ? 
O25 B4 O8 114.0(6) . . ? 
O27 B4 O8 108.0(5) . . ? 
O6 B4 O8 107.9(5) 2_677 . ? 
O25 B4 K2 58.4(3) . 1_565 ? 
O27 B4 K2 56.3(3) . 1_565 ? 
O6 B4 K2 148.4(4) 2_677 1_565 ? 
O8 B4 K2 103.4(4) . 1_565 ? 
O25 B4 K2 103.3(4) . 2_677 ? 
O27 B4 K2 48.7(3) . 2_677 ? 
O6 B4 K2 65.0(3) 2_677 2_677 ? 
O8 B4 K2 141.5(4) . 2_677 ? 
K2 B4 K2 87.7(2) 1_565 2_677 ? 
O27 B5 O19 123.1(6) . . ? 
O27 B5 O26 118.9(6) . . ? 
O19 B5 O26 118.0(6) . . ? 
O27 B5 K2 56.8(4) . 2_677 ? 
O19 B5 K2 136.9(5) . 2_677 ? 
O26 B5 K2 78.4(4) . 2_677 ? 
O27 B5 K1 131.8(5) . 2_677 ? 
O19 B5 K1 55.0(4) . 2_677 ? 
O26 B5 K1 83.2(4) . 2_677 ? 
K2 B5 K1 91.7(2) 2_677 2_677 ? 
O27 B5 K2 47.5(3) . 1_565 ? 
O19 B5 K2 124.3(5) . 1_565 ? 
O26 B5 K2 98.0(4) . 1_565 ? 
K2 B5 K2 88.5(2) 2_677 1_565 ? 
K1 B5 K2 178.8(3) 2_677 1_565 ? 
O20 B6 O14 110.9(6) . . ? 
O20 B6 O19 108.2(5) . . ? 
O14 B6 O19 107.9(6) . . ? 
O20 B6 O8 112.3(6) . . ? 
O14 B6 O8 108.3(5) . . ? 
O19 B6 O8 109.1(5) . . ? 
O20 B6 K1 105.0(4) . 2_677 ? 
O14 B6 K1 59.2(3) . 2_677 ? 
O19 B6 K1 53.4(3) . 2_677 ? 
O8 B6 K1 142.5(4) . 2_677 ? 
O20 B7 O16 110.2(5) . . ? 
O20 B7 O21 107.8(5) . . ? 
O16 B7 O21 109.7(6) . . ? 
O20 B7 O7 112.6(6) . . ? 
O16 B7 O7 107.9(5) . . ? 
O21 B7 O7 108.6(5) . . ? 
O21 B8 O30 118.4(7) . . ? 
O21 B8 O29 123.0(7) . . ? 
O30 B8 O29 118.7(7) . . ? 
O21 B8 K5 127.0(5) . . ? 
O30 B8 K5 88.5(5) . . ? 
O29 B8 K5 55.4(4) . . ? 
O23 B9 O12 111.3(6) . . ? 
O23 B9 O29 106.9(5) . . ? 
O12 B9 O29 109.8(6) . . ? 
O23 B9 O7 113.0(6) . . ? 
O12 B9 O7 108.0(5) . . ? 
O29 B9 O7 107.9(5) . . ? 
K2 O5W K3 106.7(9) . . ? 
O8W' O8W K5 102.8(12) . 2 ? 
O8W O8W' K2 132.4(15) . 1_444 ? 
O9W' O9W K3 110(4) . . ? 
O9W' O9W K4 97(6) . 1_655 ? 
K3 O9W K4 114.9(9) . 1_655 ? 
O9W O9W' K3 57(4) . . ? 
O9W O9W' K4 72(5) . 1_655 ? 
K3 O9W' K4 103.1(6) . 1_655 ? 
O10B O10A K3 118(2) . 2_666 ? 
K5 O11B K4 89.7(7) . . ? 
O12W O11A K4 88.3(17) 1_455 . ? 
O11A O12W K4 64.1(15) 1_655 1_655 ? 
 
_diffrn_measured_fraction_theta_max    0.982 
_diffrn_reflns_theta_full              25.10 
_diffrn_measured_fraction_theta_full   0.982 
_refine_diff_density_max    2.300 
_refine_diff_density_min   -2.300 
_refine_diff_density_rms    0.201 
